A continuum model of fracture that describes, in principle, the propagation and interaction of arbitrary distributions of cracks and voids with evolving topology without a “fracture criterion” is developed. It involves a “law of motion” for crack tips, primarily as a kinematical consequence coupled with thermodynamics. Fundamental kinematics endow the crack tip with a topological charge. This allows the association of a kinematical conservation law for the charge, resulting in a fundamental evolution equation for the crack-tip field and, in turn, the crack field. The vectorial crack field degrades the elastic modulus in a physically justified anisotropic manner. The mathematical structure of this conservation law allows an additive “free” gradient of a scalar field in the evolution of the crack field. We associate this naturally emerging scalar field with the porosity that arises in the modeling of ductile failure. Thus, porosity-rate gradients affect the evolution of the crack field, which then naturally degrades the elastic modulus, and it is through this fundamental mechanism that spatial gradients in porosity growth affect the strain energy density and the stress-carrying capacity of the material and, as a dimensional consequence related to fundamental kinematics, introduce a length scale in the model. A key result of this work is that brittle fracture is energy-driven while ductile fracture is stress-driven. Under overall shear loadings where the mean stress vanishes or is compressive, the shear strain energy can still drive shear fracture in ductile materials.

Revised:

Accepted:

Published online:

Amit Acharya ^{1}

@article{CRMECA_2020__348_4_275_0, author = {Amit Acharya}, title = {A possible link between brittle and ductile failure by viewing fracture as a topological defect}, journal = {Comptes Rendus. M\'ecanique}, pages = {275--284}, publisher = {Acad\'emie des sciences, Paris}, volume = {348}, number = {4}, year = {2020}, doi = {10.5802/crmeca.14}, language = {en}, }

TY - JOUR AU - Amit Acharya TI - A possible link between brittle and ductile failure by viewing fracture as a topological defect JO - Comptes Rendus. Mécanique PY - 2020 SP - 275 EP - 284 VL - 348 IS - 4 PB - Académie des sciences, Paris DO - 10.5802/crmeca.14 LA - en ID - CRMECA_2020__348_4_275_0 ER -

Amit Acharya. A possible link between brittle and ductile failure by viewing fracture as a topological defect. Comptes Rendus. Mécanique, Volume 348 (2020) no. 4, pp. 275-284. doi : 10.5802/crmeca.14. https://comptes-rendus.academie-sciences.fr/mecanique/articles/10.5802/crmeca.14/

[1] A nonlinear anisotropic elastic–inelastic constitutive model for polycrystalline ceramics and minerals with application to boron carbide, Int. J. Solids Struct., Volume 64 (2015), pp. 191-207 | DOI

[2] Experiments on fracture trajectories in ceramic samples with voids, J. Eur. Ceram. Soc., Volume 36 (2016) no. 9, pp. 2277-2281 | DOI

[3] Failure of metals I: Brittle and ductile fracture, Acta Mater., Volume 107 (2016), pp. 424-483 | DOI

[4] Fracture mechanism maps in stress space, Acta Metall., Volume 36 (1988) no. 5, pp. 1213-1228 | DOI

[5] 2D and 3D visualization of ductile fracture, Adv. Eng. Mater., Volume 8 (2006) no. 6, pp. 469-472 | DOI

[6] Ductile fracture by hole growth in shear bands, Int. J. Fract. Mech., Volume 2 (1966) no. 4, pp. 614-627 | DOI

[7] Fracture and singularities of the mass-density gradient field, J. Elast., Volume 132 (2018) no. 2, pp. 243-260 | DOI | MR | Zbl

[8] Modification of the Gurson model for shear failure, Eur. J. Mech. A, Volume 27 (2008) no. 1, p. 1 | DOI | Zbl

[9] Ductile failure modeling, Int. J. Fract., Volume 201 (2016) no. 1, pp. 29-80 | DOI

[10] A study of conditions for dislocation nucleation in coarser-than-atomistic scale models, J. Mech. Phys. Solids, Volume 75 (2015), pp. 76-92 | DOI

[11] Numerical experiments in revisited brittle fracture, J. Mech. Phys. Solids, Volume 48 (2000) no. 4, pp. 797-826 | DOI | MR | Zbl

[12] A phase-field description of dynamic brittle fracture, Comput. Methods Appl. Mech. Eng., Volume 217 (2012), pp. 77-95 | DOI | MR | Zbl

[13] Micromechanics: Overall Properties of Heterogeneous Materials, Elsevier, 2013

[14] Self-consistent analysis of waves in rocks containing arrays of cracks, Seismic Anisotropy, Society of Exploration Geophysicists, 1996, pp. 318-356 | DOI

[15] Behaviour of voids in a shear field, Int. J. Fract., Volume 158 (2009) no. 1, pp. 41-49 | DOI | Zbl

[16] Laws of crack motion and phase-field models of fracture, J. Mech. Phys. Solids, Volume 57 (2009) no. 2, pp. 342-368 | DOI | Zbl

[17] A phase field model for rate-independent crack propagation: Robust algorithmic implementation based on operator splits, Comput. Methods Appl. Mech. Eng., Volume 199 (2010) no. 45, pp. 2765-2778 | DOI | MR | Zbl

[18] Regularized formulation of the variational brittle fracture with unilateral contact: numerical experiments, J. Mech. Phys. Solids, Volume 57 (2009) no. 8, pp. 1209-1229 | DOI | Zbl

[19] A coupled crystal plasticity FEM and phase-field model for crack evolution in microstructures of 7000 series aluminum alloys, Eng. Fract. Mech., Volume 230 (2020), 106970 | DOI

[20] Plasticity aspects of fracture, Engineering Fundamentals and Environmental Effects (H. Leibowitz, ed.), Elsevier, 1971, pp. 47-225 | DOI

[21] Fracture characteristics of three metals subjected to various strains, strain rates, temperatures and pressures, Eng. Fract. Mech., Volume 21 (1985) no. 1, pp. 31-48 | DOI

[22] On fracture locus in the equivalent strain and stress triaxiality space, Int. J. Mech. Sci., Volume 46 (2004) no. 1, pp. 81-98 | DOI

[23] Rupture mechanisms in combined tension and shear—experiments, Int. J. Solids Struct., Volume 44 (2007) no. 6, pp. 1768-1786 | DOI | Zbl

[24] Constitutive modeling of void shearing effect in ductile fracture of porous materials, Eng. Fract. Mech., Volume 75 (2008) no. 11, pp. 3343-3366 | DOI

[25] A homogenization-based damage model for stiffness loss in ductile metal-matrix composites, J. Mech. Phys. Solids, Volume 137 (2020), 103812 | DOI | MR

[26] Nonlinear composites, Advances in Applied Mechanics, Volume 34, Elsevier, 1997, pp. 171-302 | DOI

[27] Finite element implementation of gradient plasticity models Part I: Gradient-dependent yield functions, Comput. Methods Appl. Mech. Eng., Volume 163 (1998) no. 1-4, pp. 11-32 | DOI | Zbl

[28] Finite element implementation of gradient plasticity models Part II: Gradient-dependent evolution equations, Comput. Methods Appl. Mech. Eng., Volume 163 (1998) no. 1-4, pp. 33-53 | DOI | Zbl

[29] Recent extensions of Gurson’s model for porous ductile metals, Continuum Micromechanics, Springer, 1997, pp. 61-130 | DOI | Zbl

[30] Collapse and coalescence of spherical voids subject to intense shearing: studied in full 3D, Int. J. Fract., Volume 177 (2012) no. 2, pp. 97-108 | DOI

[31] Application of a model of plastic porous materials including void shape effects to the prediction of ductile failure under shear-dominated loadings, J. Mech. Phys. Solids, Volume 94 (2016), pp. 148-166 | DOI | MR

[32] Phase-field modelling of ductile fracture: a variational gradient-extended plasticity-damage theory and its micromorphic regularization, Phil. Trans. R. Soc. A, Volume 374 (2016) no. 2066, 20150170 | DOI | MR | Zbl

[33] Phase-field modeling of ductile fracture, Comput. Mech., Volume 55 (2015) no. 5, pp. 1017-1040 | DOI | MR | Zbl

*Cited by Sources: *

Comments - Politique